LMucko/crystallography-open-database huggingface dataset:
Kristallstruktur von Pd9Te4
Matkovic, P.; Schubert, K.; Journal of the Less-Common Metals 58 (1978) P39–P46; doi:10.1016/0022-5088(78)90205-9

data_9012388
_publ_section_title
;
 Kristallstruktur von Pd9Te4
;
_journal_name_full               'Journal of the Less-Common Metals'
_journal_page_first              P39
_journal_page_last               P46
_journal_paper_doi               10.1016/0022-5088(78)90205-9
_journal_volume                  58
_journal_year                    1978
_chemical_formula_sum            'Pd9 Te4'
_chemical_name_mineral           Telluropalladinite
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 91.97
_cell_angle_gamma                90
_cell_length_a                   7.458
_cell_length_b                   13.938
_cell_length_c                   8.839
_cell_formula_units_Z            4
_cell_volume                     918.267
_database_code_amcsd             0014141
_exptl_crystal_density_diffrn    10.620
_cod_database_code               9012388
Kristallstrukturen von Pd2PbBi und Pd4PbBi3
Mayer, H. W.; Bhatt, Y. C.; Schubert, K.; Journal of the Less-Common Metals 66 (1979) 1–9; doi:10.1016/0022-5088(79)90189-9

data_9012389
_publ_section_title
;
 Kristallstrukturen von Pd2PbBi und Pd4PbBi3
;
_journal_name_full               'Journal of the Less-Common Metals'
_journal_page_first              1
_journal_page_last               9
_journal_paper_doi               10.1016/0022-5088(79)90189-9
_journal_volume                  66
_journal_year                    1979
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Bi Pb Pd2'
_chemical_name_mineral           Polarite
_space_group_IT_number           36
_symmetry_space_group_name_Hall  'C 2c -2c'
_symmetry_space_group_name_H-M   'C c m 21'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   7.150
_cell_length_b                   8.681
_cell_length_c                   10.535
_cell_formula_units_Z            8
_cell_volume                     653.898
_database_code_amcsd             0014143
_exptl_crystal_density_diffrn    12.779
_cod_original_formula_sum        'Pd2 Pb Bi'
_cod_database_code               9012389
Kristallstrukturen von Pd2PbBi und Pd4PbBi3
Mayer, H. W.; Bhatt, Y. C.; Schubert, K.; Journal of the Less-Common Metals 66 (1979) 1–9; doi:10.1016/0022-5088(79)90189-9

data_9012390
_publ_section_title
;
 Kristallstrukturen von Pd2PbBi und Pd4PbBi3
;
_journal_name_full               'Journal of the Less-Common Metals'
_journal_page_first              1
_journal_page_last               9
_journal_paper_doi               10.1016/0022-5088(79)90189-9
_journal_volume                  66
_journal_year                    1979
_chemical_formula_structural     Pd2PbBi
_chemical_formula_sum            'Bi Pb Pd2'
_space_group_IT_number           8
_symmetry_space_group_name_Hall  'C -2y'
_symmetry_space_group_name_H-M   'C 1 m 1'
_cell_angle_alpha                90
_cell_angle_beta                 71.74
_cell_angle_gamma                90
_cell_length_a                   7.171
_cell_length_b                   8.677
_cell_length_c                   5.575
_cell_formula_units_Z            4
_cell_volume                     329.424
_database_code_amcsd             0014144
_exptl_crystal_density_diffrn    12.683
_cod_original_formula_sum        'Pd2 Pb Bi'
_cod_database_code               9012390
_amcsd_formula_title             Pd2PbBi
Rh12As7, a host structure for rare earth elements: Crystal structures of Rh12As7 and Ho2Rh12As7 Locality: synthetic Note: x(RhII) corrected
Pivan, J. Y.; Guerin, R.; Sergent, M.; Journal of the Less-Common Metals 107 (1985) 249–258; doi:10.1016/0022-5088(85)90084-0

data_9012391
_publ_section_title
;Rh12As7, a host structure for rare earth elements: Crystal structures of
 Rh12As7 and Ho2Rh12As7 Locality: synthetic Note: x(RhII) corrected
;
_journal_name_full               'Journal of the Less-Common Metals'
_journal_page_first              249
_journal_page_last               258
_journal_paper_doi               10.1016/0022-5088(85)90084-0
_journal_volume                  107
_journal_year                    1985
_chemical_compound_source        Synthetic
_chemical_formula_sum            'As3.5 Rh6'
_chemical_name_mineral           Polkanovite
_space_group_IT_number           176
_symmetry_space_group_name_Hall  '-P 6c'
_symmetry_space_group_name_H-M   'P 63/m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   9.297
_cell_length_b                   9.297
_cell_length_c                   3.657
_cell_formula_units_Z            2
_cell_volume                     273.742
_database_code_amcsd             0014151
_exptl_crystal_density_diffrn    10.672
_cod_original_formula_sum        'Rh6 As3.5'
_cod_database_code               9012391
Synthesis and characterization of the layered metal TlCu2S2
Berger, R.; Journal of the Less-Common Metals 147 (1989) 141–148; doi:10.1016/0022-5088(89)90157-4

data_9012392
_publ_section_title
;
 Synthesis and characterization of the layered metal TlCu2S2
;
_journal_name_full               'Journal of the Less-Common Metals'
_journal_page_first              141
_journal_page_last               148
_journal_paper_doi               10.1016/0022-5088(89)90157-4
_journal_volume                  147
_journal_year                    1989
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Cu2 S2 Tl'
_chemical_name_mineral           Thalcusite
_space_group_IT_number           139
_symmetry_space_group_name_Hall  '-I 4 2'
_symmetry_space_group_name_H-M   'I 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.7771
_cell_length_b                   3.7771
_cell_length_c                   13.3791
_cell_formula_units_Z            2
_cell_volume                     190.873
_database_code_amcsd             0014164
_exptl_crystal_density_diffrn    6.883
_cod_original_formula_sum        'Tl Cu2 S2'
_cod_database_code               9012392
Rh12As7, a host structure for rare earth elements: Crystal structures of Rh12As7 and Ho2Rh12As7
Pivan, J. Y.; Guerin, R.; Sergent, M.; Journal of the Less-Common Metals 107 (1985) 249–258; doi:10.1016/0022-5088(85)90084-0

data_9012393
_publ_section_title
;
 Rh12As7, a host structure for rare earth elements: Crystal structures of
 Rh12As7 and Ho2Rh12As7
;
_journal_name_full               'Journal of the Less-Common Metals'
_journal_page_first              249
_journal_page_last               258
_journal_paper_doi               10.1016/0022-5088(85)90084-0
_journal_volume                  107
_journal_year                    1985
_chemical_formula_structural     Ho2Rh12As7
_chemical_formula_sum            'As3.5 Ho Rh6'
_space_group_IT_number           176
_symmetry_space_group_name_Hall  '-P 6c'
_symmetry_space_group_name_H-M   'P 63/m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   9.892
_cell_length_b                   9.892
_cell_length_c                   3.859
_cell_formula_units_Z            2
_cell_volume                     327.019
_database_code_amcsd             0014152
_exptl_crystal_density_diffrn    10.608
_cod_original_cell_volume        327.020
_cod_original_formula_sum        'Ho Rh6 As3.5'
_cod_database_code               9012393
_amcsd_formula_title             Ho2Rh12As7
Crystal structure of Rh12As7
Lambert-Andron B; Dhahri, E.; Chaudouet, P.; Madar, R.; Journal of the Less-Common Metals 108 (1985) 353–358; doi:10.1016/0022-5088(85)90230-9

data_9012394
_publ_section_title
;
 Crystal structure of Rh12As7
;
_journal_name_full               'Journal of the Less-Common Metals'
_journal_page_first              353
_journal_page_last               358
_journal_paper_doi               10.1016/0022-5088(85)90230-9
_journal_volume                  108
_journal_year                    1985
_chemical_compound_source        Synthetic
_chemical_formula_sum            'As3.5 Rh6'
_chemical_name_mineral           Polkanovite
_space_group_IT_number           176
_symmetry_space_group_name_Hall  '-P 6c'
_symmetry_space_group_name_H-M   'P 63/m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   9.315
_cell_length_b                   9.315
_cell_length_c                   3.659
_cell_formula_units_Z            2
_cell_volume                     274.953
_database_code_amcsd             0014153
_exptl_crystal_density_diffrn    10.625
_cod_original_formula_sum        'Rh6 As3.5'
_cod_database_code               9012394
Yafsoanite: a garnet type calcium-tellurium(VI)-zinc oxide
Jarosch, D.; Zemann, J.; Mineralogy and Petrology 40 (1989) 111–116; doi:10.1007/BF01164321

data_9012395
_publ_section_title
;
 Yafsoanite: a garnet type calcium-tellurium(VI)-zinc oxide
;
_journal_name_full               'Mineralogy and Petrology'
_journal_page_first              111
_journal_page_last               116
_journal_paper_doi               10.1007/BF01164321
_journal_volume                  40
_journal_year                    1989
_chemical_compound_source        'Aldan, USSR'
_chemical_formula_sum            'Ca3 O12 Te2 Zn3'
_chemical_name_mineral           Yafsoanite
_space_group_IT_number           230
_symmetry_space_group_name_Hall  '-I 4bd 2c 3'
_symmetry_space_group_name_H-M   'I a -3 d'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   12.632
_cell_length_b                   12.632
_cell_length_c                   12.632
_cell_formula_units_Z            8
_cell_volume                     2015.656
_database_code_amcsd             0014623
_exptl_crystal_density_diffrn    5.033
_cod_original_sg_symbol_H-M      'I a 3 d'
_cod_original_formula_sum        'Ca3 Te2 Zn3 O12'
_cod_database_code               9012395
Joesmithite, a plumbous amphibole revisited and comments on bond valences
Moore, P. B.; Davis, A. M.; Van Derveer, D. G.; Sen Gutpa, P. K.; Mineralogy and Petrology 48 (1993) 97–113; doi:10.1007/BF01163090

data_9012396
_publ_section_title
;
 Joesmithite, a plumbous amphibole revisited and comments on bond valences
;
_journal_name_full               'Mineralogy and Petrology'
_journal_page_first              97
_journal_page_last               113
_journal_paper_doi               10.1007/BF01163090
_journal_volume                  48
_journal_year                    1993
_chemical_compound_source        'Langban, Sweden'
_chemical_formula_sum
'Be1.694 Ca1.9 Fe2.449 H2 K0.072 Mg2.551 Na0.1 O24 Pb0.928 Si6.306'
_chemical_name_mineral           Joesmithite
_space_group_IT_number           13
_symmetry_space_group_name_Hall  '-P 2ya'
_symmetry_space_group_name_H-M   'P 1 2/a 1'
_cell_angle_alpha                90
_cell_angle_beta                 105.95
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   9.915
_cell_length_b                   17.951
_cell_length_c                   5.243
_cell_volume                     897.246
_database_code_amcsd             0014625
_exptl_crystal_density_diffrn    3.889
_cod_original_formula_sum
'(Pb.928 K.072) Mg2.551 Fe2.449 (Ca1.9 Na.1) Si6.306 Be1.694 O24 H2'
_cod_database_code               9012396
Bellbergite - a new mineral with the zeolite structure type EAB
Ruedinger, B.; Tillmanns, E.; Hentschel, G.; Mineralogy and Petrology 48 (1993) 147–152; doi:10.1007/BF01163093

data_9012397
_publ_section_title
;
 Bellbergite - a new mineral with the zeolite structure type EAB
;
_journal_name_full               'Mineralogy and Petrology'
_journal_page_first              147
_journal_page_last               152
_journal_paper_doi               10.1007/BF01163093
_journal_volume                  48
_journal_year                    1993
_chemical_formula_sum            'Al9 Ca3 H33.388 K O51 Si9 Sr'
_chemical_name_mineral           Bellbergite
_space_group_IT_number           194
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   13.224
_cell_length_b                   13.224
_cell_length_c                   15.988
_cell_volume                     2421.310
_exptl_crystal_density_diffrn    2.184
_cod_original_formula_sum        'K Sr Ca3 (Al9 Si9) O51 H33.388'
_cod_database_code               9012397
_cod_duplicate_entry 9009840
On zeophyllite from Radejcin, Ceske stredohori Mts.: X-ray and IR-investigations Locality: Alter Berg, Radzein Note: z-coordinate of Si2 was changed from 0.70304 to 0.07304 to match reported bond lengths
Mikenda, W.; Pertlik, F.; Povondra, P.; Ulrych, J.; Mineralogy and Petrology 61 (1997) 199–209; doi:10.1007/BF01172484

data_9012398
_publ_section_title
;On zeophyllite from Radejcin, Ceske stredohori Mts.: X-ray and
 IR-investigations Locality: Alter Berg, Radzein Note: z-coordinate of Si2 was
 changed from 0.70304 to 0.07304 to match reported bond lengths
;
_journal_name_full               'Mineralogy and Petrology'
_journal_page_first              199
_journal_page_last               209
_journal_paper_doi               10.1007/BF01172484
_journal_volume                  61
_journal_year                    1997
_chemical_compound_source        'Alter Berg, Radzein'
_chemical_formula_sum            'Ca13 F10 H12 O34 Si10'
_chemical_name_mineral           Zeophyllite
_space_group_IT_number           148
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   9.377
_cell_length_b                   9.377
_cell_length_c                   36.57
_cell_volume                     2784.732
_database_code_amcsd             0014639
_exptl_crystal_density_diffrn    2.769
_cod_original_sg_symbol_H-M      'R -3'
_cod_original_formula_sum        'Ca13 Si10 O34 F10 H12'
_cod_database_code               9012398
Niedermayrite, Cu4Cd(SO4)2(OH)6*4H2O, a new mineral from the Lavrion Mining District, Greece Locality: Lavrion mining district, Attica peninsula, Greece
Giester, G.; Rieck, B.; Brandstatter, F.; Mineralogy and Petrology 63 (1998) 19–34; doi:10.1007/BF01162766

data_9012399
_publ_section_title
;Niedermayrite, Cu4Cd(SO4)2(OH)6*4H2O, a new mineral from the Lavrion Mining
 District, Greece Locality: Lavrion mining district, Attica peninsula, Greece
;
_journal_name_full               'Mineralogy and Petrology'
_journal_page_first              19
_journal_page_last               34
_journal_paper_doi               10.1007/BF01162766
_journal_volume                  63
_journal_year                    1998
_chemical_compound_source
'Lavrion mining district, Attica peninsula, Greece'
_chemical_formula_sum            'Cd Cu4 H14 O18 S2'
_chemical_name_mineral           Niedermayrite
_space_group_IT_number           11
_symmetry_space_group_name_Hall  '-P 2yb'
_symmetry_space_group_name_H-M   'P 1 21/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 92.04
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.543
_cell_length_b                   21.995
_cell_length_c                   6.079
_cell_volume                     740.672
_database_code_amcsd             0014641
_exptl_crystal_density_diffrn    3.286
_cod_original_formula_sum        'Cu4 Cd S2 O18 H14'
_cod_database_code               9012399
Johntomaite, a new member of the bjarebyite group of barium phosphates: description and structure refinement Locality: Spring Creek copper mine, southern Flinders Ranges, South Australia
Kolitsch, U.; Pring, A.; Tiekink, E. R. T.; Mineralogy and Petrology 70 (2000) 1–14; doi:10.1007/s007100070009

data_9012400
_publ_section_title
;Johntomaite, a new member of the bjarebyite group of barium phosphates:
 description and structure refinement Locality: Spring Creek copper mine,
 southern Flinders Ranges, South Australia
;
_journal_name_full               'Mineralogy and Petrology'
_journal_page_first              1
_journal_page_last               14
_journal_paper_doi               10.1007/s007100070009
_journal_volume                  70
_journal_year                    2000
_chemical_compound_source
'Spring Creek copper mine, southern Flinders Ranges, South Australia'
_chemical_formula_sum            'Ba Ca0.3 Fe3.7 H3 O15 P3'
_chemical_name_mineral           Johntomaite
_space_group_IT_number           11
_symmetry_space_group_name_Hall  '-P 2yb'
_symmetry_space_group_name_H-M   'P 1 21/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 100.21
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   9.200
_cell_length_b                   12.369
_cell_length_c                   5.003
_cell_volume                     560.300
_database_code_amcsd             0014643
_exptl_crystal_density_diffrn    4.101
_cod_original_formula_sum        'Ba Fe3.7 Ca.3 P3 O15 H3'
_cod_database_code               9012400
The crystal structure of nesquehonite, MgCO3*3H2O, from Lavrion, Greece
Giester, G.; Lengauer, C. L.; Rieck, B.; Mineralogy and Petrology 70 (2000) 153–163; doi:10.1007/s007100070001

data_9012401
_publ_section_title
;
 The crystal structure of nesquehonite, MgCO3*3H2O, from Lavrion, Greece
;
_journal_name_full               'Mineralogy and Petrology'
_journal_page_first              153
_journal_page_last               163
_journal_paper_doi               10.1007/s007100070001
_journal_volume                  70
_journal_year                    2000
_chemical_compound_source        'Sounion, Lavrion mining district, Greece'
_chemical_formula_sum            'C H6 Mg O6'
_chemical_name_mineral           Nesquehonite
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_cell_angle_alpha                90
_cell_angle_beta                 90.41
_cell_angle_gamma                90
_cell_length_a                   7.701
_cell_length_b                   5.365
_cell_length_c                   12.126
_cell_formula_units_Z            4
_cell_volume                     500.983
_database_code_amcsd             0014644
_exptl_crystal_density_diffrn    1.834
_cod_original_formula_sum        'Mg C O6 H6'
_cod_database_code               9012401
Leogangite, Cu10(AsO4)4(SO4)(OH)6*8H2O, a new mineral from the Leogang mining district, Salzburg province, Austria Locality: Leogang polymetallic ore district, Salzburg province, Austria
Lengauer, C. L.; Giester, G.; Kirchner, E.; Mineralogy and Petrology 81 (2004) 187–201; doi:10.1007/s00710-004-0032-x

data_9012402
_publ_section_title
;Leogangite, Cu10(AsO4)4(SO4)(OH)6*8H2O, a new mineral from the Leogang mining
 district, Salzburg province, Austria Locality: Leogang polymetallic ore
 district, Salzburg province, Austria
;
_journal_name_full               'Mineralogy and Petrology'
_journal_page_first              187
_journal_page_last               201
_journal_paper_doi               10.1007/s00710-004-0032-x
_journal_volume                  81
_journal_year                    2004
_chemical_compound_source
'Leogang polymetallic ore district, Salzburg province, Austria'
_chemical_formula_sum            'As4 Cu10 H22 O34 S'
_chemical_name_mineral           Leogangite
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 92.85
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   21.770
_cell_length_b                   12.327
_cell_length_c                   10.720
_cell_volume                     2873.248
_database_code_amcsd             0014647
_exptl_crystal_density_diffrn    3.545
_cod_original_formula_sum        'Cu10 As4 S O34 H22'
_cod_database_code               9012402
Garavellite, FeSbBiS4, from the Caspari mine, North Rhine-Westphalia, Germany: composition, physical properties and determination of the crystal structure Locality: Caspari mine, North Rhine-Westphalia, Germany
Bindi, L.; Menchetti, S.; Mineralogy and Petrology 85 (2005) 131–139; doi:10.1007/s00710-005-0083-7

data_9012403
_publ_section_title
;Garavellite, FeSbBiS4, from the Caspari mine, North Rhine-Westphalia,
 Germany: composition, physical properties and determination of the crystal
 structure Locality: Caspari mine, North Rhine-Westphalia, Germany
;
_journal_name_full               'Mineralogy and Petrology'
_journal_page_first              131
_journal_page_last               139
_journal_paper_doi               10.1007/s00710-005-0083-7
_journal_volume                  85
_journal_year                    2005
_chemical_compound_source
'Caspari mine, North Rhine-Westphalia, Germany'
_chemical_formula_sum            'Bi Fe S4 Sb'
_chemical_name_mineral           Garavellite
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2c 2n'
_symmetry_space_group_name_H-M   'P n a m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   11.413
_cell_length_b                   14.164
_cell_length_c                   3.759
_cell_formula_units_Z            4
_cell_volume                     607.656
_database_code_amcsd             0014648
_exptl_crystal_density_diffrn    5.628
_cod_original_formula_sum        'Fe Sb Bi S4'
_cod_database_code               9012403
Hexagonal close packed krypton and xenon Sample: at T = 26 K
Sonnenblick, Y.; Alexander, E.; Kalman, Z. H.; Steinberger, I. T.; Chemical Physics Letters 52 (1977) 276–278; doi:10.1016/0009-2614(77)80540-X

data_9012404
_publ_section_title
;
 Hexagonal close packed krypton and xenon
 Sample: at T = 26 K
;
_journal_name_full               'Chemical Physics Letters'
_journal_page_first              276
_journal_page_last               278
_journal_paper_doi               10.1016/0009-2614(77)80540-X
_journal_volume                  52
_journal_year                    1977
_chemical_compound_source        Synthetic
_chemical_formula_sum            Kr
_chemical_name_common            Krypton
_chemical_name_mineral           Krypton
_space_group_IT_number           194
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.00
_cell_length_b                   4.00
_cell_length_c                   6.53
_cell_formula_units_Z            2
_cell_volume                     90.482
_database_code_amcsd             0012190
_diffrn_ambient_temperature      26
_exptl_crystal_density_diffrn    3.076
_cod_database_code               9012404